J Adv Prosthodont 2016;8:267-74
Shear bond strength of indirect composite material to monolithic zirconia Fatih Sari1, Asli Secilmis1*, Irfan Simsek2, Semih Ozsevik3 Department of Prosthodontics, Faculty of Dentistry, University of Gaziantep, Gaziantep, Turkey Department of Prosthodontics, Faculty of Dentistry, University of Adiyaman, Adiyaman, Turkey 3 Department of Restorative Dentistry, Faculty of Dentistry, University of Gaziantep, Gaziantep, Turkey 1 2
PURPOSE. This study aimed to evaluate the effect of surface treatments on bond strength of indirect composite material (Tescera Indirect Composite System) to monolithic zirconia (inCoris TZI). MATERIALS AND METHODS. Partially stabilized monolithic zirconia blocks were cut into with 2.0 mm thickness. Sintered zirconia specimens were divided into different surface treatment groups: no treatment (control), sandblasting, glaze layer & hydrofluoric acid application, and sandblasting + glaze layer & hydrofluoric acid application. The indirect composite material was applied to the surface of the monolithic zirconia specimens. Shear bond strength value of each specimen was evaluated after thermocycling. The fractured surface of each specimen was examined with a stereomicroscope and a scanning electron microscope to assess the failure types. The data were analyzed using one-way analysis of variance (ANOVA) and Tukey LSD tests (α=.05). RESULTS. Bond strength was significantly lower in untreated specimens than in sandblasted specimens (P 45%) Silane (> 1%)
Bisco Inc., Schaumburg, IL, USA
Porcelain Bonding Resin
HEMA-Free, hydrophobic bonding resin
Bis-GMA (30-50%) UDMA (30-50%) TEGDMA (10-30%)
Bisco Inc., Schaumburg, IL, USA
Tescera Indirect Composite System
Reinforced microfill composite (Body)
Ethoxylated Bis-GMA (< 15%) UDMA (< 15%) Glass filler (< 80%) Amorphous silica (< 25%)
Bisco Dental Product Asia Ltd., Seoul, Korea
MDP: 10-methacryloyloxydecyl dihydrogen phosphate, BPDM: Biphenyldimethacriylate, Bis-GMA: Bisphenol A diglycidylethermethacrylate, UDMA: Urethane dimethacrylate, TEGDMA: Triethylene glycol dimethacrylate
a feldspathic glazing ceramic powder (65% silica, 15% alumina, 10% sodyum oxide, 5% potassium oxide, and 5% titanium oxide) mixed with stain liquid (Vita Akzent Plus; Vita Zahnfabrik, Bad Säckingen, Germany) was carefully applied as a thin coat using a ceramic brush and allowed to air-dry. The specimens were heated up to 750°C and fired for 20 minutes using a computer-programmed electrical induction furnace (Programat P300; IvoclarVivadent AG, Liechtenstein, Austria) then cooled at room temperature. Then, the specimens were conditioned with HF (9% PorcEtch; Reliance Ortho Prod. Inc., Itasca, IL, USA) for 90 seconds and rinsed with water for 30 seconds. Sandblasting + Glaze layer & HF application group (SG): The surfaces of specimens were sandblasted as mentioned above, cleaned ultrasonically for 10 minutes and dried. After, glaze layer & HF application was performed on the surfaces as noted above. The surface of monolithic zirconia specimens for control (C) and sandblasting (S) groups was treated with 1 coat of Z-Prime Plus (Bisco Inc., Schaumburg, IL, USA), uniformly wetting the surface and oil-free air was gently blown for 3-5 seconds. However, in glaze layer & HF application (G) and sandblasting + glaze layer & HF application (SG) groups, a thin layer of Porcelain Primer (Bisco Inc., Schaumburg, IL, USA) was applied to monolithic zirconia surfaces according to the manufacturer’ recommendation. Then, Porcelain Bonding Resin (Bisco Inc., Schaumburg, IL, USA) was applied for 10 seconds, with oil-free air gently blown across the surface to evaporate the solvent, and photo-cured for 10 seconds (Valo Cordless; Ultradent Products Inc., South Jordan, UT, USA). A silicon tubes with a hole in the center (3.2 mm in internal diameter and 3 mm in height) was placed on the specimen surface and incrementally filled with reinforced
microfill composite (Tescera Indirect Composite System, Body; Bisco Inc., Schaumburg, IL, USA). The light source (Valo Cordless; Ultradent Products Inc., South Jordan, UT, USA) was positioned to be in contact with the fluid path and the indirect composite material was photo-cured at 20 seconds. After, specimens were polymerized under pressure and light during approximately 2 minutes using Tescera ATL Light Cup (Bisco Inc., Schaumburg, IL, USA). Final polymerization was completed during 10-13 minutes using Tescera ATL Pressure/Light/Heat Cure Cup (Bisco Inc., Schaumburg, IL, USA). All specimens were subjected to 1000 cycles of thermal cycling in deionized water from 5°C to 55°C, with 30 seconds dwelling and 15 seconds transfer times (SD Mechatronic Ther mocycler; SD Mechatronic GmbH, Westerham, Germany). SBS was determined using a universal testing machine (Shimadzu AG-X, Shimadzu Corporation, Kyoto, Japan). A knife-edge shearing rod at a crosshead speed of 0.5 mm/ min was used on the bond interface. Maximum shear load at the point of failure was recorded. SBS (σ) was calculated using the load at failure (F) and the adhesive area (A): σ=F/ A (N/mm2). New specimens were prepared to evaluate changes in surface topography after surface treatment. The specimens were sputter-coated with gold/palladium (Polaron, Emitech Ltd., Kent, UK) and examined with a SEM (JSM-6060LV, Jeol, Tokyo, Japan) (×1000). Moreover, the fractured surfaces of the monolithic zirconia specimens were examined with a stereomicroscope (Leica model, Leica QWinV.3 software, Leica Microsystem Imaging Solutions, Cambridge, UK) (×10) and scanning electron microscope (×25, ×350 and ×1000) after the SBS test. Failure types were classified as adhesive (at the monolithic zirconia-indirect composite The Journal of Advanced Prosthodontics
J Adv Prosthodont 2016;8:267-74
material interface), cohesive (within the monolithic zirconia or indirect composite material), or mixed. In cases of mixed failure, the surface of the monolithic zirconia material was partially covered by the remaining indirect composite and/or adhesive material. Data were analyzed using SPSS for Windows version 22.0 (SPSS Inc., Chicago, IL, USA). The normal distribution of data was firstly checked and verified using the Kolmogorov Smirnov test. One-way analysis of variance (ANOVA) and Tukey LSD tests were used, where P < .05 was accepted as significant.
RESULTS The one-way ANOVA test indicated that the difference among the groups was statistically significant (P < .05). Table 2 displays the mean SBS values and standard deviations for all groups. There were statistically significant differences among the groups (P < .05), except G and SG
groups (P > .05). The results of failure type assessments after SBS test are summarized in Table 2. Mixed failure was observed in tested groups, excepting the C and S groups in which both adhesive and mixed failures were observed. Cohesive failures of the monolithic zirconia or indirect composite material failures were not found. Fig. 1A shows the SEM image of specimen in control group characterized by a relatively smooth surface. There were marks occur in the surface of the specimen during cutting and grinding. After sandblasting, the zirconia surface was uniformly rougher and exhibited surface textures with sharp edges and shallow pits (Fig. 1B). The specimens of the G and SG groups exhibited different images from other groups. SEM images of these specimens displayed the formation of micropores at different widths and depths, due to the dissolution of glass matrix depending on the HF application (Fig. 1C and Fig. 1D). Fig. 2A show SEM image of the surface applied
Table 2. The groups of study, the results of shear bond strength test (MPa) and failure type Surface treatment
Z-Prime Plus Porcelain Primer + Porcelain Bonding Resin
Sandblasting + Glaze layer & HF application
Porcelain Primer + Porcelain Bonding Resin
Glaze layer & HF application
Control (No treatment)
Tescera Indirect Composite System
Mean (SD) 0.92 (0.69)A
Same uppercase letters were not significantly different at P < .05. SD: Standard deviation.
Fig. 1. SEM micrographs of monolithic zirconia specimens: (A) control, (B) sandblasting, (C) glaze layer & HF application, (D) sandblasting + glaze layer & HF application.
Shear bond strength of indirect composite material to monolithic zirconia
Z-Prime Plus after grinding. No scratches generated by the abrasive papers can be seen. In the C group, the SEM images of the fracture interface revealed remains of the priming agent and the indirect composite material on the surface of specimen (Fig. 2B and Fig. 2C). Figs. 3A and 3B are SEM images of the sandblasted group after SBS test. The remnants of adhered material on the surface of the specimen indicated mixed failure observed. Both of glaze layer & HF application treated groups exhibited mixed type of the failure (Fig. 3C and Fig. 3D).
DISCUSSION The present study aimed to estimate the availability of indirect composite material veneered monolithic zirconia prostheses. The null hypothesis that different surface treatments have no effect on indirect composite material-monolithic zirconia bond strength was rejected. In the present study,
the G and SG groups had significantly higher bond strengths than the other two groups. However, there was no significant difference in bond strength between the G and SG groups. Previous studies have shown that indirect composite material produced low bonding strength values when applied to untreated zirconia ceramic surfaces.23 The effect of priming agent on the bond strength of indirect composite material to zirconia ceramic has also been evaluated19-21 and it has been reported that it could increase the bond strength.18,21 In the groups G and SG, since the glass phase was created on the surface, Porcelain Primer and Porcelain Bonding Resin were applied to the surfaces while Z-Prime Plus was applied to the monolithic zirconia specimens in the C and S groups according to the manufacturer’s instructions. In this study, untreated monolithic zirconia specimens used to determine the effect of the priming agent and this group
Fig. 2. (A) SEM micrograph of monolithic zirconia specimen applied Z-Prime Plus, (B) control group exhibited mixed failure, (C) in the surface of a specimen from the control group, both monolithic zirconia and remnants of Z-Prime Plus and indirect composite material were visible.
Fig. 3. SEM micrographs of monolithic zirconia specimens. (A) sandblasted group exhibited mixed failure, (B) remnants of Z-Prime Plus and indirect composite material were seen in the surface of sandblasted specimen, (C) glaze layer & HF application group exhibited mixed failure, (D) in the glaze layer & HF application group, the indirect composite material on the monolithic zirconia was observed. The Journal of Advanced Prosthodontics
J Adv Prosthodont 2016;8:267-74
had the lowest bond strength. Sandblasting creates surface roughness by cleaning the surface of framework and increases the mechanical or chemical bond strength between metal or other substrates and composite material.21 There were significant differences in bond strength between C and S groups in present study. The bond strength value was higher after sandblasting. According to this result, it can be said that sandblasting significantly affects bond strength and producing a stable bond without appropriate surface treatment may be difficult. This was due to a synergistic effect produced by the increased contact area on the chemical interactions between the 10-methacryloyloxydecyl dihydrogen phosphate (MDP) and carboxylic monomers of the Z-Prime Plus and the monolithic zirconia surface. The reported data of the present study on the effect of the sandblasting and priming agent application on bond strength is in agreement with previous studies.18,20,28 The MDP monomer has a phosphoric acid group which can be bonded to hydroxyl groups in the zirconia surface and a carboxylic acid group will bond to composite resin.35 Z-Prime Plus is an MDP-containing primer and applied one or two coats without being specific about light polymerization according to the manufacturer’s instructions. In a previous study, Seabra et al.35 reported that the higher bond strength was obtained with applying 2 coats of Z-Prime Plus followed by light polymerization compared to the other groups. In present study, one coat of primer was applied and it was not light-polymerized. Organofunctionalsilanes contain 2 different reactive functional groups that can react and couple with various inorganic and organic materials. They are used as adhesion promoters, increasing the union of dissimilar materials. The reaction of hydrolysable functional groups to the surface hydroxyl groups of inorganic substrates creates a siloxane bond. Organic functional groups react with functional groups of resins.36,37 The glaze layer & HF application on monolithic zirconia surface followed by silanization have resulted in a significantly improved bond with indirect composite material. This result is associated with formation of strong chemical bonds between the silane and the silica in the porcelain.20 This data was confirmed by the findings of previous studies.20,33 In the present study, a thin layer of low-fusing porcelain was applied to monolithic zirconia surfaces for G and SG groups and specimens were fired. Results of the present study revealed that this procedure, regardless of application of sandblasting, is able to provide a more retentive surface than sandblasted monolithic zirconia. This reasoning is further supported by the prevalence of mixed failures in G and SG groups. Moreover, it can be said that sandblasting before glaze layer & HF application does not enhance the extra micromechanical interlocking. The data for SBS test were supported by the SEM images. SEM image of S group showed a unique corrugated appearance as shown in previous studies.20,21,23 This corrugated appearance is considered to indicate the phenomenon 272
of strong adhesion to resist the shear force. This seems to have been a result of the sandblasting rather than the priming agent although the results showed that the bond strength significantly increased compared with the C group. Glaze layer & HF application groups exhibit numerous micropores at different widths and depths, due to the dissolution of glass matrix depending on the HF treatment that was applied. This view is similar to the study of Fushiki et al.20. In present study, in the groups with the lower SBS values (C and S groups) a few adhesive failures were found, whereas in the groups with higher SBS values (G and SG), only mixed type failures were observed. In G and SG groups, the monolithic zirconia surface is covered with more indirect composite material than the other two groups (C and S). This result is a sign of generating strong adhesion by etched glaze layer. In vitro studies are necessary for understanding the laboratory performances of materials. However, they are not sound criteria for the prediction of their clinical efficacy. Further studies may be required to compare complete restorations and the effects of mechanical load cycling in artificial saliva. Controlled long-term clinical studies are needed to confirm the success of treatment procedures.
CONCLUSION Within the limitation of this in vitro study, the following conclusions can be drawn: The glaze layer & HF application provides high bond strength between indirect composite material (Tescera Indirect Composite System) and monolithic zirconia (inCoris TZI). Indirect composite materials may be a promising alternative as a veneering material for monolithic zirconia restorations.
ORCID Fatih Sari http://orcid.org/0000-0002-4818-8562 Asli Secilmis http://orcid.org/0000-0002-1065-3262 Irfan Simsek http://orcid.org/0000-0002-4524-1129 Semih Ozsevik http://orcid.org/0000-0001-9818-4853
REFERENCES 1. Oliveira-Ogliari A, Collares FM, Feitosa VP, Sauro S, Ogliari FA, Moraes RR. Methacrylate bonding to zirconia by in situ silica nanoparticle surface deposition. Dent Mater 2015;31: 68-76. 2. Preis V, Letsch C, Handel G, Behr M, Schneider-Feyrer S, Rosentritt M. Influence of substructure design, veneer application technique, and firing regime on the in vitro performance of molar zirconia crowns. Dent Mater 2013;29:e11321. 3. Raigrodski AJ, Yu A, Chiche GJ, Hochstedler JL, Mancl LA, Mohamed SE. Clinical efficacy of veneered zirconium dioxide-based posterior partial fixed dental prostheses: five-year results. J Prosthet Dent 2012;108:214-22.
Shear bond strength of indirect composite material to monolithic zirconia
4. Worni A, Kolgeci L, Rentsch-Kollar A, Katsoulis J, MericskeStern R. Zirconia-based screw-retained prostheses supported by implants: a retrospective study on technical complications and failures. Clin Implant Dent Relat Res 2015;17:1073-81. 5. Tartaglia GM, Sidoti E, Sforza C. Seven-year prospective clinical study on zirconia-based single crowns and fixed dental prostheses. Clin Oral Investig 2015;19:1137-45. 6. Monaco C, Caldari M, Scotti R; AIOP (Italian Academy of Prosthetic Dentistry) Clinical Research Group. Clinical evaluation of zirconia-based restorations on implants: a retrospective cohort study from the AIOP clinical research group. Int J Prosthodont 2015;28:239-42. 7. Sadid-Zadeh R, Liu PR, Aponte-Wesson R, O’Neal SJ. Maxillary cement retained implant supported monolithic zirconia prosthesis in a full mouth rehabilitation: a clinical report. J Adv Prosthodont 2013;5:209-17. 8. Moscovitch M. Consecutive case series of monolithic and minimally veneered zirconia restorations on teeth and implants: up to 68 months. Int J Periodontics Restorative Dent 2015;35:315-23. 9. Nakamura K, Harada A, Inagaki R, Kanno T, Niwano Y, Milleding P, Örtengren U. Fracture resistance of monolithic zirconia molar crowns with reduced thickness. Acta Odontol Scand 2015;73:602-8. 10. Venezia P, Torsello F, Cavalcanti R, D’Amato S. Retrospective analysis of 26 complete-arch implant-supported monolithic zirconia prostheses with feldspathic porcelain veneering limited to the facial surface. J Prosthet Dent 2015;114:506-12. 11. Rinke S, Fischer C. Range of indications for translucent zirconia modifications: clinical and technical aspects. Quintessence Int 2013;44:557-66. 12. Matsuzaki F, Sekine H, Honma S, Takanashi T, Furuya K, Yajima Y, Yoshinari M. Translucency and flexural strength of monolithic translucent zirconia and porcelain-layered zirconia. Dent Mater J 2015;34:910-7. 13. Vichi A, Carrabba M, Paravina R, Ferrari M. Translucency of ceramic materials for CEREC CAD/CAM system. J Esthet Restor Dent 2014;26:224-31. 14. Preis V, Schmalzbauer M, Bougeard D, Schneider-Feyrer S, Rosentritt M. Surface properties of monolithic zirconia after dental adjustment treatments and in vitro wear simulation. J Dent 2015;43:133-9. 15. Ramos GF, Monteiro EB, Bottino MA, Zhang Y, Marques de Melo R. Failure probability of three designs of zirconia crowns. Int J Periodontics Restorative Dent 2015;35:843-9. 16. Lee SY, Vang MS, Yang HS, Park SW, Park HO, Lim HP. Shear bond strength of composite resin to titanium according to various surface treatments. J Adv Prosthodont 2009;1: 68-74. 17. Kanat B, Cömlekoğlu EM, Dündar-Çömlekoğlu M, Hakan Sen B, Ozcan M, Ali Güngör M. Effect of various veneering techniques on mechanical strength of computer-controlled zirconia framework designs. J Prosthodont 2014;23:445-55. 18. Kobayashi K, Komine F, Blatz MB, Saito A, Koizumi H, Matsumura H. Influence of priming agents on the shortterm bond strength of an indirect composite veneering material to zirconium dioxide ceramic. Quintessence Int 2009;40:
545-51. 19. Komine F, Fushiki R, Koizuka M, Taguchi K, Kamio S, Matsumura H. Effect of surface treatment on bond strength between an indirect composite material and a zirconia framework. J Oral Sci 2012;54:39-46. 20. Fushiki R, Komine F, Blatz MB, Koizuka M, Taguchi K, Matsumura H. Shear bond strength between an indirect composite layering material and feldspathic porcelain-coated zirconia ceramics. Clin Oral Investig 2012;16:1401-11. 21. Koizuka M, Komine F, Blatz MB, Fushiki R, Taguchi K, Matsumura H. The effect of different surface treatments on the bond strength of a gingiva-colored indirect composite veneering material to three implant framework materials. Clin Oral Implants Res 2013;24:977-84. 22. Komine F, Taguchi K, Fushiki R, Kamio S, Iwasaki T, Matsumura H. In vitro comparison of fracture load of implant-supported, zirconia-based, porcelain- and compositelayered restorations after artificial aging. Dent Mater J 2014; 33:607-13. 23. Su N, Yue L, Liao Y, Liu W, Zhang H, Li X, Wang H, Shen J. The effect of various sandblasting conditions on surface changes of dental zirconia and shear bond strength between zirconia core and indirect composite resin. J Adv Prosthodont 2015;7:214-23. Erratum in: J Adv Prosthodont 2015;7:506. 24. Kakaboura A, Rahiotis C, Zinelis S, Al-Dhamadi YA, Silikas N, Watts DC. In vitro characterization of two laboratoryprocessed resin composites. Dent Mater 2003;19:393-8. 25. Cetin AR, Unlu N, Cobanoglu N. A five-year clinical evaluation of direct nanofilled and indirect composite resin restorations in posterior teeth. Oper Dent 2013;38:E1-11. 26. Ozakar-Ilday N, Zorba YO, Yildiz M, Erdem V, Seven N, Demirbuga S. Three-year clinical performance of two indirect composite inlays compared to direct composite restorations. Med Oral Patol Oral Cir Bucal 2013;18:e521-8. 27. Fruits TJ, Knapp JA, Khajotia SS. Microleakage in the proximal walls of direct and indirect posterior resin slot restorations. Oper Dent 2006;31:719-27. 28. Yi YA, Ahn JS, Park YJ, Jun SH, Lee IB, Cho BH, Son HH, Seo DG. The effect of sandblasting and different primers on shear bond strength between yttria-tetragonal zirconia polycrystal ceramic and a self-adhesive resin cement. Oper Dent. 2015;40:63-71. 29. Karakoca S, Yilmaz H. Influence of surface treatments on surface roughness, phase transformation, and biaxial flexural strength of Y-TZP ceramics. J Biomed Mater Res B Appl Biomater 2009;91:930-7. 30. Gargari M, Gloria F, Napoli E, Pujia AM. Zirconia: cementation of prosthetic restorations. Literature review. Oral Implantol (Rome) 2010;3:25-9. 31. Erdem A, Akar GC, Erdem A, Kose T. Effects of different surface treatments on bond strength between resin cements and zirconia ceramics. Oper Dent 2014;39:E118-27. 32. Cura C, Özcan M, Isik G, Saracoglu A. Comparison of alternative adhesive cementation concepts for zirconia ceramic: glaze layer vs zirconia primer. J Adhes Dent 2012;14:75-82. 33. Everson P, Addison O, Palin WM, Burke FJ. Improved bonding of zirconia substructures to resin using a “glaze-on” The Journal of Advanced Prosthodontics
J Adv Prosthodont 2016;8:267-74
technique. J Dent 2012;40:347-51. 34. Bottino MA, Bergoli C, Lima EG, Marocho SM, Souza RO, Valandro LF. Bonding of Y-TZP to dentin: effects of Y-TZP surface conditioning, resin cement type, and aging. Oper Dent 2014;39:291-300. 35. Seabra B, Arantes-Oliveira S, Portugal J. Influence of multimode universal adhesives and zirconia primer application techniques on zirconia repair. J Prosthet Dent 2014;112:1827. 36. Lung CY, Matinlinna JP. Aspects of silane coupling agents and surface conditioning in dentistry: an overview. Dent Mater 2012;28:467-77. 37. Lung CY, Liu D, Matinlinna JP. Silica coating of zirconia by silicon nitride hydrolysis on adhesion promotion of resin to zirconia. Mater Sci Eng C Mater Biol Appl 2015;46:103-10.